Seeing Luminescence Appear as Crystals Crumble. Isolation and Subsequent Self-Association of Individual [(C6H11NC)2Au]+ Ions in Crystals.
Luong, Lucy M. C.; Lowe, Christopher D.; Adams, Alexandria V.; Moshayedi, Venoos; Olmstead, Marilyn M.; Balch, Alan L.; Chemical Science  (2020) –; doi:10.1039/D0SC03299A

data_1559047
_publ_section_title
;
 Seeing Luminescence Appear as Crystals Crumble. Isolation and Subsequent
 Self-Association of Individual [(C6H11NC)2Au]+&#x00A0;Ions in Crystals.
;
_journal_name_full               'Chemical Science'
_journal_paper_doi               10.1039/D0SC03299A
_journal_year                    2020
_chemical_formula_moiety         'C14 H22 Au N2, C6 H6, F6 Sb'
_chemical_formula_sum            'C20 H28 Au F6 N2 Sb'
_chemical_formula_weight         729.16
_chemical_name_common            C6H6\^A.[(C6H11NC)2Au]SbF6
_chemical_properties_physical    Air-sensitive
_space_group_crystal_system      tetragonal
_space_group_IT_number           128
_space_group_name_Hall           '-P 4 2n'
_space_group_name_H-M_alt        'P 4/m n c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-06-13 deposited with the CCDC.	2020-09-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.948(4)
_cell_length_b                   12.948(4)
_cell_length_c                   13.943(4)
_cell_measurement_reflns_used    3481
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      26.3045
_cell_measurement_theta_min      2.918
_cell_volume                     2337.6(12)
_computing_cell_refinement       'SAINT (Bruker, 2017)'
_computing_data_collection       'Apex3 (Bruker, 2017)'
_computing_data_reduction        'SAINT (Bruker, 2017)'
_computing_publication_material  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 10.42
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker Kappa DUO with Photon 100'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0342
_diffrn_reflns_av_unetI/netI     0.0219
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            8037
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.386
_diffrn_reflns_theta_min         2.146
_diffrn_source                   microsource
_exptl_absorpt_coefficient_mu    7.481
_exptl_absorpt_correction_T_max  0.99983
_exptl_absorpt_correction_T_min  0.99847
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick,2016)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.072
_exptl_crystal_description       block
_exptl_crystal_F_000             1384
_exptl_crystal_recrystallization_method
'Re-crystallisation from solvent: benzene'
_exptl_crystal_size_max          0.506
_exptl_crystal_size_mid          0.044
_exptl_crystal_size_min          0.042
_refine_diff_density_max         1.567
_refine_diff_density_min         -1.028
_refine_diff_density_rms         0.142
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.168
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     85
_refine_ls_number_reflns         1251
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.167
_refine_ls_R_factor_all          0.0568
_refine_ls_R_factor_gt           0.0357
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0460P)^2^+5.1186P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0848
_refine_ls_wR_factor_ref         0.0946
_reflns_Friedel_coverage         0.000
_reflns_number_gt                887
_reflns_number_total             1251
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0sc03299a2.cif
_cod_data_source_block           ll113
_cod_original_cell_volume        2337.6(14)
_cod_database_code               1559047
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.116
_shelx_estimated_absorpt_t_max   0.744
_shelx_res_checksum              85555